Structures and properties of a BEDT-TTF-based organic charge transfer salt and the zwitterion of ferrocenesulfonate.
Akutsu, Hiroki; Yamada, Jun-Ichi; Nakatsuji, Shin'ichi; Turner, Scott S.; Dalton transactions (Cambridge, England : 2003) 42 (2013) 16351–16354; doi:10.1039/c3dt52346b

data_7024000
_publ_section_title
;
 Structures and properties of a BEDT-TTF-based organic charge transfer
 salt and the zwitterion of ferrocenesulfonate.
;
_journal_issue                   46
_journal_name_full
'Dalton transactions (Cambridge, England : 2003)'
_journal_page_first              16351
_journal_page_last               16354
_journal_paper_doi               10.1039/c3dt52346b
_journal_volume                  42
_journal_year                    2013
_chemical_formula_moiety         'C10 H9 Fe O3 S'
_chemical_formula_sum            'C10 H9 Fe O3 S'
_chemical_formula_weight         265.09
_space_group_IT_number           14
_symmetry_cell_setting           monoclinic
_symmetry_Int_Tables_number      14
_symmetry_space_group_name_Hall  '-P 2yn'
_symmetry_space_group_name_H-M   'P 1 21/n 1'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_cell_angle_alpha                90.0000
_cell_angle_beta                 95.638(5)
_cell_angle_gamma                90.0000
_cell_formula_units_Z            4
_cell_length_a                   7.731(2)
_cell_length_b                   13.150(3)
_cell_length_c                   9.828(3)
_cell_measurement_reflns_used    3012
_cell_measurement_temperature    295
_cell_measurement_theta_max      29.98
_cell_measurement_theta_min      2.08
_cell_volume                     994.3(5)
_computing_cell_refinement       CrystalClear
_computing_data_collection       'CrystalClear (Rigaku Inc., 2008)'
_computing_data_reduction        CrystalClear
_computing_molecular_graphics    'CrystalStructure 4.0'
_computing_publication_material  'CrystalStructure 4.0 (Rigaku, 2010)'
_computing_structure_refinement  'SHELXL97 (Sheldrick, 2008)'
_computing_structure_solution    'Il Milione (Burla, et al., 2007)'
_diffrn_ambient_temperature      295
_diffrn_detector_area_resol_mean 7.314
_diffrn_measured_fraction_theta_full 0.996
_diffrn_measured_fraction_theta_max 0.996
_diffrn_measurement_device_type  'Rigaku Mercury70'
_diffrn_measurement_method       \w
_diffrn_radiation_type           'Mo K\a'
_diffrn_radiation_wavelength     0.71075
_diffrn_reflns_av_R_equivalents  0.0555
_diffrn_reflns_limit_h_max       10
_diffrn_reflns_limit_h_min       -10
_diffrn_reflns_limit_k_max       12
_diffrn_reflns_limit_k_min       -17
_diffrn_reflns_limit_l_max       12
_diffrn_reflns_limit_l_min       -10
_diffrn_reflns_number            8116
_diffrn_reflns_theta_full        27.50
_diffrn_reflns_theta_max         27.50
_diffrn_standards_number         0
_exptl_absorpt_coefficient_mu    1.704
_exptl_absorpt_correction_T_max  0.873
_exptl_absorpt_correction_T_min  0.835
_exptl_absorpt_correction_type   numerical
_exptl_absorpt_process_details   'NUMABS (Rigaku, 1999)'
_exptl_crystal_colour            black
_exptl_crystal_density_diffrn    1.771
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       prism
_exptl_crystal_F_000             540.00
_exptl_crystal_size_max          0.120
_exptl_crystal_size_mid          0.100
_exptl_crystal_size_min          0.080
_refine_diff_density_max         0.910
_refine_diff_density_min         -0.390
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.051
_refine_ls_hydrogen_treatment    constr
_refine_ls_number_parameters     136
_refine_ls_number_reflns         2269
_refine_ls_number_restraints     0
_refine_ls_R_factor_gt           0.0352
_refine_ls_shift/su_max          0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w = 1/[\s^2^(Fo^2^)+(0.0629P)^2^+0.0000P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_ref         0.1000
_reflns_number_gt                1942
_reflns_number_total             2272
_reflns_threshold_expression     F^2^>2.0\s(F^2^)
_cod_data_source_file            c3dt52346b.txt
_cod_data_source_block           V121106a
_cod_original_cell_volume        994.4(5)
_cod_database_code               7024000